Abstract
In this study, a numerical modeling approach was used to investigate the currentvoltage behavior of conductive nanoplateletbased nanocomposites. A threedimensional continuum Monte Carlo model was employed to randomly disperse the nanoplatelets in a cubic representative volume element. A nonlinear finite elementbased model was developed to evaluate the electrical behavior of the nanocomposite for different levels of the applied electric field. Also, the effect of filler loading on nonlinear conductivity behavior of nanocomposites was investigated. The validity of the developed model was verified through qualitative comparison of the simulation results with results obtained from experimental works.
Keywords:
Nanocomposites; Conductive nanoplatelets; Currentvoltage characteristicsBackground
In recent years, the nonlinear electrical conductivity behavior of nanoparticlemodified polymers has received considerable attention by researchers, and several studies have been carried out to investigate the currentvoltage characteristics of conductive nanocomposites. Even though several studies investigated the nonohmic conductivity behavior of insulator polymers filled with conductive spherical and sticklike inclusions [15], to the best of the authors' knowledge, all of the research in this field has been limited to experimental works. Experimental research devoted to the electric properties of nanoplateletbased nanocomposites investigated the electrical conductivity of polymers with exfoliated graphite sheets with sizes varying from a few microns to several hundreds of a micron [610], which allows for only limited prediction of the conductivity behavior of nanocomposites with submicron size inclusions.
These limitations motivated the present authors to conduct a numerical study to investigate the currentvoltage behavior of polymers made electrically conductive through the uniform dispersion of conductive nanoplatelets. Specifically, the nonlinear electrical characteristics of conductive nanoplateletbased nanocomposites were investigated in the present study. Threedimensional continuum Monte Carlo modeling was employed to simulate electrically conductive nanocomposites. To evaluate the electrical properties, the conductive nanoplatelets were assumed to create resistor networks inside a representative volume element (RVE), which was modeled using a threedimensional nonlinear finite element approach. In this manner, the effect of the voltage level on the nanocomposite electrical behavior such as electrical resistivity was investigated.
Methods
Monte Carlo modeling
Theoretically, a nanocomposite is rendered electrically conductive by inclusions dispersed inside the polymer that form a conductive path through which an electrical current can pass. Such a path is usually termed a percolation network. Figure 1 illustrates the conductivity mechanism of an insulator polymer made conductive through the formation of a percolation network. In this figure, elements in black, white, and gray color indicate nanoplatelets that are individually dispersed, belong to an electrically connected cluster, or form a percolation network inside the RVE, respectively. Quantum tunneling of electrons through the insulator matrix is the dominant mechanism in the electric behavior of conductive nanocomposites. Figure 2 illustrates the concept of a tunneling resistor for simulating electron tunneling through an insulator matrix and its role in the formation of a percolation network.
Figure 1. Schematic of a representative volume element illustrating nanoplatelets (black), clusters (white), and percolation network (gray).
Figure 2. Illustration of tunneling resistors.
Electron tunneling through a potential barrier exhibits different behaviors for different voltage levels, and thus, the percolation behavior of a polymer reinforced by conductive particles is governed by the level of the applied voltage. In a low voltage range (eV ≈ 0), the tunneling resistivity is approximately proportional to the insulator thickness, that is, the tunneling resistivity shows ohmic behavior [11]. For higher voltages, however, the tunneling resistance is no longer constant for a given insulator thickness, and it has been shown to depend on the applied voltage level. It was derived by Simmons [11] that the electrical current density passing through an insulator is given by
where
J_{0} = e/2πh(βΔs)^{2} and
Considering Equation 1, even for comparatively low voltage levels, the current density passing through the insulator matrix is nonlinearly dependent on the electric field. For vanishing voltages, when eV ≈ 0, Equation 1 can be simplified as [11]
The numerical evaluation of Equation 1 given in Figure 3 shows the resistivity per unit area of polymer with 4nm thickness and a quantum tunneling barrier height λ of 1 eV, with respect to the normalized voltage eV/λ. This graph indicates that a polymer only exhibits close to ohmic behavior when subjected to low electric fields, that is, the resistivity of the polymer is approximately constant in a small region near the ordinate axis (see inset in Figure 3), permitting the use of the linear approximation provided by Equation 2.
Figure 3. Polymer resistivity per unit area versus normalized voltage. The inset shows approximately ohmic behavior for low electric fields.
In this study, a rectangular potential barrier was assumed to model the electrical behavior of the tunneling resistor. Tunneling resistivity is numerically evaluated for λ = 0.5 ev employing Equation 2 and illustrated in Figure 4. The tunneling resistance is drastically dependent on the insulator thickness, that is, tunneling resistance is sharply increasing as the insulator thickness is increasing. A cutoff distance can therefore be approximated at which tunneling resistors with length greater than this threshold do not appreciably contribute toward the overall conductivity of the nanocomposite. In [12] and [13], the cutoff distance was assumed to be 1.0 and 1.4 nm, respectively. It is expected that the resistivity of the insulator film is decreasing as the electrical field is increasing; so, when dealing with higher voltage levels, tunneling resistors with length greater than these cutoff distances may play a role in the nanocomposite conductivity. Hence, it was conservatively assumed in this study that tunneling resistors with length less than 4 nm contribute toward the nanocomposite conductivity.
Figure 4. Tunneling resistivity versus insulator thickness.
In the first step of this work, a threedimensional continuum percolation model based on Monte Carlo simulation was used to study the percolation behavior of an insulator matrix reinforced with conductive nanoplatelet fillers. Additional details on this modeling approach can be found in an earlier publication [14]. In the simulation, circular nanoplatelets are randomly generated and added to the RVE. The shortest distance between adjacent particles is calculated, and particles with distance between them shorter than the cutoff distance are grouped into clusters. The formation of a cluster connecting two parallel faces of the RVE is considered the formation of a percolation network that allows electric current to pass through the RVE, rendering it conductive.
Finite element modeling
To study the electrical properties of nanocomposites, in particular their conductivity behavior, the employed modeling approach further involved the creation of a nonlinear threedimensional finite element resistor network. Considering the excellent conductivity of the considered nanoplatelets (e.g. σ = 10^{8} S/m for graphene), the electrical potential drop across the nanoplatelets was neglected. The tunneling resistors were modeled as nonohmic, which resistivity is governed by Equation 1. Employing appropriate finite element formulations, the governing equation of an electrical resistor can be written as
where I_{ij} is the electrical current passing between the ith and jth node; k_{ij} is the conductance of the resistor between nodes i and j; and V_{i} is the voltage of the ith node measured with respect to a node connected to ground. The system of the nonlinear equations governing the electrical behavior of the nanocomposite was obtained by assembling the governing equations for the individual elements. The resulting nonlinear system of equations was solved employing an iterative method.
Results and discussion
Modeling results
The developed model was employed to investigate the electrical behavior of a polymer with λ = 0.5 ev made conductive through the uniform dispersion of conductive circular nanoplatelets with a diameter of 100 nm. In the simulations, the size of the RVE was chosen to be nine times the diameter of the nanodisks, which was ascertained to be large enough to minimize finite size effects. In an earlier study [15], the authors showed that the Monte Carlo simulation results are no longer appreciably RVEsize dependent when the RVE size is about eight times the sum of 2R + d_{t}, where R and d_{t} are the radius of the nanoplatelets and tunneling distance, respectively.The graph in Figure 5 depicts the effect of filler loading on nanocomposite conductivity. As expected, a critical volume fraction indicated by a sharp increase in nanocomposite conductivity, i.e., the percolation threshold, can be inferred from the graph.In the following, electric current densities passing through the nanocomposite RVE were computed for different electric field levels and filler volume fractions. As illustrated by Figure 6, the current density versus voltage curves were found to be nonlinear. The depicted electrical behavior of the conductive nanocomposite is thus clearly governed by the applied voltage in a nonohmic manner, which, as mentioned above, matches the expectation for a conductive nanocomposite at higher electric field levels.
Figure 5. Conductivity of nanocomposite with respect to filler loading of conductive nanodisks with diameter of 100 nm.
Figure 6. Electric current density of nanocomposites with 100nmdiameter nanoplatelets versus the applied electrical field.
Figure 7 shows the variation of resistivity as a function of the applied electric field E in order to compare the nonohmic behavior for nanocomposites with different filler loadings. Note that resistivity values were normalized with respect to a reference resistivity measured at E = 0.8 V/cm. The results as displayed in Figure 7 indicate that the magnitude of the applied electric field plays an important role in the conductivity of nanoplateletbased nanocomposites. The employed modeling approach predicts nanocomposite resistivity to be a nonlinear function of the applied voltage. Clearly, the nanocomposites exhibit nonohmic behavior where the resistivity decreases with increasing voltage. Interestingly, the results in Figure 7 also indicate a reduced drop in resistivity and decreased nonohmic behavior for nanocomposites with higher filler volume fraction, that is, nanocomposites with higher filler loadings are less sensitive to the applied electric field level.
Figure 7. Normalized resistivity of nanocomposites with 100nm nanodisks as a function of the applied electrical field.
Comparison with experimental data
To corroborate the simulation results, conductive epoxy nanocomposite samples were produced by in situ polymerization and their electrical behavior assessed as illustrated by Figure 8. BisphenolA epoxy resin and nonMDA polyamine curing agent (EPON 826 and EPIKURE 9551, by Hexion Specialty Chemicals, Columbus, Ohio, USA) were used for the fabrication of samples that were made electrically conductive by dispersing graphene nanoplatelets (xGnPM25, by XG Sciences, Lansing, Michigan, USA).
Figure 8. Normalized resistivity data versus applied electrical field from experiments with nanographene/epoxy samples.
Graphene nanoplatelets were dispersed in acetone by sonication using a probe sonicater in an ice bath. In the following, epoxy was added to the mixture and sonication was repeated. The solvent was evaporated by heating the mixture on a magnetic stir plate and stirring with a Tefloncoated magnet. Remaining acetone was removed by using a vacuum chamber. The curing agent was added to the mixture and mixed with a highspeed mechanical shear mixer. The mixture was again degassed using the vacuum chamber and subsequently poured into a mold. A 2h cure cycle was then performed at 120°C. Resulting samples were machined into circular disks with 30mm diameter and 3mm thickness. The sample volume resistivities were measured at different applied voltages employing a Keithley 6517A electrometer connected to a Keithley test fixture (Keithley Instruments, Cleveland, Ohio, USA).Data in Figure 8 depicting the resistivity behavior of the epoxy nanocomposite samples was normalized with respect to the resistivity measured at an applied voltage of 10 V. Samples with 1 and 1.25% graphene volume fraction exhibited high resistivity levels indicating a filler loading below the percolation threshold. For higher graphene volume fractions of 1.75 and 2.25%, measurements indicated that percolation was achieved, and resistivity was found to decrease with the increase of the applied electric field. As predicted by the preceding modeling work, sample resistivity was found to be less sensitive to the applied electrical field for higher filler loadings. Hence, modeling and simulation results are qualitatively in good agreement, indicating the validity of the assumptions undertaken for the numerical modeling. However, the data presented in Figures 7 and 8 also signify that further studies are warranted to establish a quantitative agreement between numerical and experimental results.
Characterization of resistivity behavior
Gorrasi et al. [5] and Liu et al. [16] showed that the resistivity of carbon nanotubebased nanocomposites as a function of the electric power P = V × I can be described by an exponential expression:
where α is an index which generally varies between −1 and 0. The value of α is indicative of the nonlinearity of the currentvoltage relationship, i.e., α = 0 corresponds to ohmic behavior, and α decreases with increasing nonlinearity of the currentvoltage curve; r is a parameter relating to the resistivity of the nanocomposite when the electrical power passing through the sample is 1 W [16].
Computed nanocomposite resistivities are displayed as a function of the electric power in the graph in Figure 9. Data obeying Equation 4 appear in the form of straight lines owing to the graph's logarithmic scale. As shown in Figure 9, the slope of the lines decreases as the nonlinearity is decreasing with increasing filler loading. The values of α as a function of filler volume fraction are provided in Figure 10. It is shown that α values are increasing with rising filler volume fraction. A discontinuity in α values can be observed in this graph for filler volume fractions of about 5%, which is associated with the percolation volume fraction. The behavior of data simulated herein is qualitatively congruent with results reported in [5] for carbon nanotube nanocomposites.
Figure 9. Resistivity of nanocomposites with 100nm circular nanoplatelets as a function of electric power.
Figure 10. Value of α as a function of filler volume fraction for nanocomposites with 100nm circular nanoplatelets.
Conclusions
In this study, the currentvoltage behavior of conductive nanoplateletbased nanocomposites was investigated. To this end, a numerical modeling approach was developed. The simulations predicted the resistivity of nanoplateletbased nanocomposites to be strongly affected by the applied electric field. The nanocomposites exhibit nonohmic behavior, that is, resistivity is a nonlinear function of the applied electric field. Further, nanocomposite resistivity was ascertained to decrease with increasing voltage, while the degree of nonlinear behavior was found to decline with rising filler volume fraction. A good qualitative agreement was observed between simulations and experimental data, the latter of which was obtained employing measurements on nanographene/epoxy nanocomposites. The qualitative agreement between numerical and experimental studies encourages conducting a more comprehensive study to establish a quantitative agreement. The analysis further revealed that nanocomposite resistivity as a function of electrical power can be described by an exponential relation, where the exponent is a measure of the deviation from nonohmic behavior of the conductive nanocomposite.
Nomenclature
d_{t}, tunneling distance
e, electron charge
E, applied electric field
h, Planck's constant
I, electrical current
J, quantum tunneling current density
k, conductance of tunneling resistor
L, dimension of representative volume element
m, electron mass
P, electric power
r, resistivity parameter
R, radius of circular nanoplatelets
s_{1}, s_{2}, limits of barrier at Fermi level
Δs = s_{2} − s_{1}
V, voltage across insulator
V_{f,} filler volume fraction
α, nonlinearity factor
β, correction factor
λ, height of barrier for quantum tunneling
ρ, electrical resistivity
σ, electrical conductivity
Competing interests
The authors declare that they have no competing interests.
Authors' contribution
All authors made equally valuable contributions to this paper. All authors read and approved the final manuscript.
Acknowledgements
This research work was supported by the following organizations: Alberta InnovatesTechnology Futures, ROSEN Swiss AG, and Syncrude Canada Ltd.
References

An S, Mahapatra DR: Quasistatic and dynamic strain sensing using carbon nanotube/epoxy nanocomposite thin films.
Smart Mater Struct 2009, 18:045013. Publisher Full Text

Wichmann M, Buschhorn S, Gehrmann J, Schulte K: Piezoresistive response of epoxy composites with carbon nanoparticles under tensile load.

Cattin C, Hubert P: Network formation and electrical conduction in carbon nanotube modified polydimethylsiloxane.

Ounaies Z, Park C, Wise KE, Siochi EJ, Harrison JS: Electrical properties of single wall carbon nanotube reinforced polyimide composites.
Compos Sci Technol 2003, 63:16371646. Publisher Full Text

Gorrasi G, Piperopoulos E, Lanza M, Milone C: Effect of morphology of the filler on the electrical behavior of poly(Llactide) nanocomposites.

Lin H, Lu W, Chen G: Nonlinear DC conduction behavior in epoxy resin/graphite nanosheets composites.
Physica B 2007, 400:229236. Publisher Full Text

Celzard A, Furdin G, Mareche JF, McRae E: Nonlinear current–voltage characteristics in anisotropic epoxy resin–graphite flake composites.
J Mater Sci 1997, 32:18491853. Publisher Full Text

Zheng Q, Song Y, Wu G, Yi X: Reversible nonlinear conduction behavior for highdensity polyethylene/graphite powder composites near the percolation threshold.
J Polym Sci Part B 2001, 39:28332842. Publisher Full Text

Chen G, Weng W, Wu D, Wu C: Nonlinear conduction in nylon6/foliated graphite nanocomposites above the percolation threshold.
J Polym Sci Part B 2004, 42:155167. Publisher Full Text

He LX, Tjong SC: Zener tunneling in conductive graphite/epoxy composites: Dielectric breakdown aspects.
Express Polym Lett 2013, 7:375382. Publisher Full Text

Simmons G: Generalized formula for the electric tunnel effect between similar electrodes separated by a thin insulating film.
J Appl Phys 1963, 34:17931803. Publisher Full Text

Hu N, Karube Y, Yan C, Masuda Z, Fukunaga H: Tunneling effect in a polymer/carbon nanotube nanocomposite strain sensor.
Acta Mater 2008, 56:29292936. Publisher Full Text

Bao WS, Meguid SA, Zhu ZH, Weng GJ: Tunneling resistance and its effect on the electrical conductivity of carbon nanotube nanocomposites.
J Appl Phys 2012, 111:093726. Publisher Full Text

Oskouyi AB, Mertiny P: Monte Carlo model for the study of percolation thresholds in composites filled with circular conductive nanodisks.

Oskouyi AB, Sundararaj U, Mertiny P: Tunneling conductivity and piezoresistivity of composites containing randomly dispersed conductive nanoplatelets.
Materials 2014, 7:25012521. Publisher Full Text

Liu CH, Fan SS: Nonlinear electrical conducting behavior of carbon nanotube networks in silicone elastomer.
Appl Phys Lett 2007, 90:041905. Publisher Full Text